An ultraviolet-visible distinguishable broadband photodetector based on the positive and negative photoconductance effects of a graphene/ZnO quantum dot heterostructure
Henan Key Laboratory of Diamond Optoelectronic Materials and Devices, Key Laboratory of Material Physics, Ministry of Education, School of Physics and Microelectronics, Zhengzhou University, Zhengzhou 450052, Henan, China.
#Authors contributed equally.
Correspondence to: Dr. Shaobo Cheng, Henan Key Laboratory of Diamond Optoelectronic Materials and Devices, Key Laboratory of Material Physics, Ministry of Education, School of Physics and Microelectronics, Zhengzhou University, Zhengzhou 450052, Henan, China. E-mail:
Broadband photodetectors covering the ultraviolet (UV) to visible range are significant for applications in communication and imaging. Broadband photodetectors with the capacity to distinguish wavelength bands are highly desirable because they can provide additional spectral information. Herein, we report a UV-visible distinguishable broadband photodetector based on a graphene/ZnO quantum dot heterostructure. The photodetector exhibits negative photoconductance under visible illumination because the adsorbents on graphene act as scattering centers to reduce the carrier mobility. In contrast, under UV illumination, the photodetector shows positive photoconductance as the photogenerated electrons in the ZnO quantum dots transfer to the graphene, thereby increasing the conductivity. Thus, the detection and distinction of UV and visible illumination can be realized by utilizing the opposing photoconductivity changes. These results offer inspiration for the design of multifunctional broadband photodetectors.
Photodetectors, which convert optical to electrical signals, play a key role in optoelectronic systems[1-6]. In contrast to photodetectors that respond only to a specific wavelength range, broadband photodetectors can detect light over a broad spectral range and it is therefore essential to various techniques, including image sensing, optical communications, environmental monitoring, and so on[7-9]. Broadband photodetectors responding to light over a wide spectral range from ultraviolet (UV) to infrared have been developed from a variety of materials, such as two-dimensional (2D) materials, perovskites, organic semiconductors, and so on. However, the specific band of the incident light usually cannot be distinguished[10-13]. Therefore, broadband photodetectors with the capacity to distinguish different wavelength bands are highly desirable and can provide additional spectral information. For instance, UV-visible distinguishable broadband photodetectors are required for astronomical detection, information storage and other applications[1,14-16]. However, it is challenging to detect and distinguish UV and visible light using a single photodetector.
Graphene is a promising material for broadband photodetectors due to its wide-range absorption spectrum and high carrier mobility[17-22]. More interestingly, both positive and negative photoconductance responses have been reported for graphene photodetectors[23-25]. Ordinarily, light with photon energy larger than the band gap generates carriers in the valence and conduction bands of a semiconductor material, thereby increasing the conductivity. Such positive photoconductance (PPC) has been observed in most photodetectors[26,27]. In contrast to PPC, the conductivity in some low-dimensional materials may decrease under illumination, i.e., negative photoconductance (NPC)[24,28-30]. This abnormal phenomenon has been observed in photodetectors based on graphene, InAs nanowires, ZnS nanoparticles, carbon nanotubes, monolayer MoS2, and so on[23,30-32]. NPC in graphene is related to surface adsorbents, which act as scattering centers and decrease the carrier mobility under light illumination, leading to a decrease in conductivity[33,34]. In contrast, graphene photodetectors with PPC and high responsivity can also be obtained from van der Waals heterostructures composed of graphene and other materials[7,35]. The opposing photoconductivity changes of photodetectors with PPC and NPC can be easily distinguished. Therefore, UV-visible distinguishable broadband photodetectors may be realized by integrating the two different response mechanisms in the same photodetector.
Here, we present a UV-visible distinguishable photodetector composed of graphene and zinc oxide (ZnO) quantum dots (QDs). Bare graphene shows NPC under illumination from the UV to visible region. To make the response in the UV and visible region distinguishable, ZnO QDs are coated onto graphene to convert the NPC response under UV illumination to a PPC response. ZnO is chosen to absorb UV illumination due to its wide bandgap (3.3 eV, ~376 nm), low cost and abundant nanostructures[37-42]. Moreover, given that the surface states of ZnO are sensitive to the environment, the applications of ZnO photodetectors may further be extended to the chemical, medical and biological fields[43-48]. In the graphene/ZnO QD van der Waals heterostructure, electrons generated in the ZnO QDs by UV light can transfer to the graphene and enhance its conductivity, resulting in PPC in the UV region. Furthermore, the graphene/ZnO QD photodetector retains the NPC response in the visible region because the ZnO QDs do not absorb visible light. In this context, the graphene/ZnO QD photodetector shows PPC under UV light and NPC under visible light, thereby realizing the detection and distinction of UV and visible illumination simultaneously.
RESULTS AND DISCUSSION
Before investigating the spectral response characteristics of the graphene/ZnO QD photodetector, we first study the photoresponsive behavior of the bare graphene device. A schematic diagram of the bare graphene photodetector is displayed in Figure 1A. In this structure, graphene functions as the charge transport channel as well as the light-absorbing medium. The Raman spectrum of graphene is shown in Figure 1B. The two predominant peaks located at 1583 and 2680 cm-1 can be attributed to the graphene G- and
Figure 1. Bare graphene photodetector. (A) Schematic diagram of device structure (device area is 100 µm in length and 1200 µm in width defined as the area between the two electrodes). (B) Raman spectrum of graphene. (C) Photoelectric on/off response under illumination in the UV to visible range (VDS = 0.2 V and VG = 0 V). (D) Responsivity at different wavelengths.
To make the response of the photodetector to UV illumination distinguishable from that to visible illumination, the graphene is coated with ZnO QDs to form a graphene/ZnO QD photodetector, as shown in Figure 2A. Figure 2B presents the transmission electron microscopy (TEM) image of the ZnO QDs, which show a typical diameter of
Figure 2. Graphene/ZnO QD heterostructure. (A) Schematic diagram of graphene/ZnO QD heterostructure. (B) TEM image of
Figure 3A shows the response characteristics of the graphene/ZnO QD photodetector under UV (upper panel) and visible (lower panel) illumination. NPC behavior can be observed under visible illumination, similar to that of the bare graphene photodetector. However, under UV illumination, the IDS increases gradually, indicating PPC response to UV illumination. After the light is switched off, the IDS recovers to its original level slowly. The current under 650 nm illumination recovers to 21% after 1400 s, while the current under 313 nm illumination recovers to 4% after 700 s. The opposing photoconductance changes under UV and visible illumination confirm the spectrum-selective detection of the graphene/ZnO QD device. Figure 3B and C show the time-dependent response curves of the graphene/ZnO QD photodetector under 365 and 460 nm illumination, respectively. The light sources are turned on and off periodically to investigate the reproducibility of the photoresponse. Both the PPC and NPC responses are repeatable. However, the baselines change slightly after multicycle testing, which may derive from catalytic modification of the graphene.
Figure 3. Graphene/ZnO QD photodetector. (A) Photocurrent response under UV and visible illumination (VDS = 0.2 V and VG = 0 V). Time-dependent photoresponse of photodetector under (B) 460 and (C) 365 nm illumination (VDS = 0.2 V and VG = 0 V).
Figure 4A and B plot the responsivity of the graphene/ZnO QD photodetector as a function of light intensity. The responsivity decreases with the light intensity and the data can be fitted using R∝Eβ-1, where E is the light intensity and β is a constant. The constant β values under visible (460 nm) and UV (365 nm) illumination are fitted to be 0.46 and 0.12, respectively. The different β values suggest different trap states for NPC under visible illumination and PPC under UV illumination.
Figure 4. Responsivity of graphene/ZnO QD photodetector as a function of light intensity for (A) 460 and (B) 365 nm illumination.
To obtain a better understanding of the response mechanism of the graphene/ZnO QD photodetector, we measured the transfer curves under UV (365 nm) and visible (460 nm) illumination, as shown in
Figure 5. Photoresponsive behavior of graphene/ZnO QD photodetector. Transfer curves under (A) 460 and (B) 365 nm illumination
Figure 5D shows the responsivity spectrum of the graphene/ZnO QD photodetector accompanied by the absorption spectrum of the ZnO QDs. The absorption edge of the ZnO QDs (376 nm) is denoted by the vertical dashed line. It is apparent that the graphene/ZnO QD photodetector shows PPC under illumination with photon energy larger than the bandgap of the ZnO QDs, because a large amount of photon-generated electrons transfer from the ZnO QDs to the graphene, thereby increasing the conductivity. Furthermore, under illumination with photon energy smaller than the bandgap of the ZnO QDs, photoinduced impurity scattering plays the leading role, resulting in NPC. Thus, in this context, the NPC response of the graphene for UV illumination can be converted to a PPC response, thereby realizing the detection and distinction of UV and visible light using a single graphene/ZnO QD photodetector.
In conclusion, we have demonstrated a UV-visible distinguishable broadband photodetector utilizing the NPC and PPC response in a graphene/ZnO QD heterostructure. The photoresponsive mechanism of the photodetector under visible illumination is attributed to adsorbents on the graphene, which act as scattering centers in illumination conditions to decrease the conductivity. In contrast, under UV illumination, the photogenerated electrons in the ZnO QDs could transfer to the graphene, leading to an increase in conductivity. Thus, the current of the graphene/ZnO QDs photodetector decreases under visible illumination and increases under UV illumination, which can be used to detect and distinguish UV and visible illumination. Our results may expand the application area of broadband photodetectors.
MATERIALS AND METHODS
Device Fabrication: Graphene was grown on copper foils via a chemical vapor deposition method and transferred to Si(n+)/SiO2 (300 nm) substrates via the solution method. Then, two Ti/Au electrodes were prepared onto the graphene by thermal evaporation using a mask. Another Ti/Au electrode was deposited on the Si substrate as a gate electrode [Figure 1A]. The device active area is 100 µm in length and 1200 µm in width defined as the area between the two electrodes. ZnO QDs were synthesized by a traditional sol-gel method using zinc acetate and KOH as reactants. To fabricate the graphene/ZnO QD photodetector, the ZnO QDs dispersed in an ethanol solution
Device Characterization: The electrical transport characteristics of the device were studied using a semiconductor characterization system (Keithley 4200-SCS). Handhold lasers and LEDs with different wavelengths were employed as the light sources. The X-ray diffraction (XRD) pattern of the ZnO QDs was obtained using a diffractometer (X’Pert Pro, PANalytical). The Raman spectra were recorded using an SOL instrument spectrometer (Confotec MR520) using a 532-nm laser as the excitation source. X-ray photoelectron spectroscopy (XPS) spectra were carried out using an XPS spectrometer
Design, writing review and editing: Yang X, Cheng S, Shan CX
Data analysis: Yang X, Yang XG, Cheng S
Data acquisition: Yang X, Wang CJ
Sample fabrication: Wang CJ, Zang JHAvailability of data and materials
Not applicable.Financial support and sponsorship
This work was supported by National Natural Science Foundation of China (Nos. 62271450, 12174348) and Henan Center for Outstanding Overseas Scientists (No. GZS201903).Conflicts of interest
All authors declared that there are no conflicts of interest.Ethical approval and consent to participate
Not applicable.Consent for publication
© The Author(s) 2023.
2. Clifford JP, Konstantatos G, Johnston KW, Hoogland S, Levina L, Sargent EH. Fast, sensitive and spectrally tuneable colloidal-quantum-dot photodetectors. Nat Nanotechnol 2009;4:40-4.
3. Patel M, Kumar M, Kim J. Polarity flipping in an isotype heterojunction (p-SnS/p-Si) to enable a broadband wavelength selective energy-efficient photodetector. J Mater Chem C 2018;6:6899-904.
4. Bao C, Yang J, Bai S, et al. High performance and stable all-inorganic metal halide perovskite-based photodetectors for optical communication applications. Adv Mater 2018;30:e1803422.
5. Li Y, Shi Z, Li X, Shan C. Photodetectors based on inorganic halide perovskites: materials and devices. Chinese Phys B 2019;28:017803.
6. Guo Q, Pospischil A, Bhuiyan M, et al. Black phosphorus mid-infrared photodetectors with high gain. Nano Lett 2016;16:4648-55.
7. Liu CH, Chang YC, Norris TB, Zhong Z. Graphene photodetectors with ultra-broadband and high responsivity at room temperature. Nat Nanotechnol 2014;9:273-8.
10. Ding N, Wu Y, Xu W, et al. A novel approach for designing efficient broadband photodetectors expanding from deep ultraviolet to near infrared. Light Sci Appl 2022;11:91.
11. Li C, Wang H, Wang F, et al. Ultrafast and broadband photodetectors based on a perovskite/organic bulk heterojunction for large-dynamic-range imaging. Light Sci Appl 2020;9:31.
13. Nanda Kumar Reddy N, Godavarthi S, Mohan Kumar K, et al. Evaluation of temperature dependent electrical transport parameters in Fe3O4/SiO2/n-Si metal-insulator-semiconductor (MIS) type Schottky barrier heterojunction in a wide temperature range. J Mater Sci Mater Electron 2019;30:8955-66.
14. Chesnokov S, Dolzhenko D, Ivanchik I, Khokhlov D. Far infrared high-performance lead telluride-based photodetectors for space-born applications. Infrared Phys Technol 1994;35:23-31.
15. Kind H, Yan HQ, Messer B, Law M, Yang PD. Nanowire ultraviolet photodetectors and optical switches. Adv Mater 2002;14:158-60.
16. Schaffer M, Mitkas P. Requirements and constraints for the design of smart photodetector arrays for page-oriented optical memories. IEEE J Select Topics Quantum Electron 1998;4:856-65.
17. Hu W, Li Q, Chen X, Lu W. Recent progress on advanced infrared photodetectors. Acta Phys Sin 2019;68:35.
18. Long M, Wang P, Fang H, Hu W. Progress, challenges, and opportunities for 2D material based photodetectors. Adv Funct Mater 2019;29:1803807.
19. Zhang X, John S. Broadband light-trapping enhancement of graphene absorptivity. Phys Rev B 2019:99.
20. Jia W, Ren P, Tian Y, Fan C. Dynamically tunable optical properties in graphene-based plasmon-induced transparency metamaterials. Chinese Phys B 2019;28:026102.
21. Xia C, Xue B, Wang T, Peng Y, Jia Y. Interlayer coupling effects on Schottky barrier in the arsenene-graphene van der Waals heterostructures. Appl Phys Lett 2015;107:193107.
22. Du H, Jia Y, Sun Q, Guo Z. Single vacancy defects diffusion at the initial stage of graphene growth: a first-principles study. Phys Lett A 2015;379:1270-3.
23. Cui B, Xing Y, Han J, et al. Negative photoconductivity in low-dimensional materials. Chinese Phys B 2021;30:028507.
24. Biswas C, Güneş F, Duong DL, et al. Negative and positive persistent photoconductance in graphene. Nano Lett 2011;11:4682-7.
25. Sun Z, Liu Z, Li J, Tai GA, Lau SP, Yan F. Infrared photodetectors based on CVD-grown graphene and PbS quantum dots with ultrahigh responsivity. Adv Mater 2012;24:5878-83.
26. Nakanishi H, Bishop KJ, Kowalczyk B, et al. Photoconductance and inverse photoconductance in films of functionalized metal nanoparticles. Nature 2009;460:371-5.
27. Hayden O, Agarwal R, Lieber CM. Nanoscale avalanche photodiodes for highly sensitive and spatially resolved photon detection. Nat Mater 2006;5:352-6.
28. Han Y, Zheng X, Fu M, et al. Negative photoconductivity of InAs nanowires. Phys Chem Chem Phys 2016;18:818-26.
29. Wei P, Chattopadhyay S, Yang M, et al. Room-temperature negative photoconductivity in degenerate InN thin films with a supergap excitation. Phys Rev B 2010:81.
30. Chen X, Xu Y, Zhou D, et al. Solar-blind photodetector with high avalanche gains and bias-tunable detecting functionality based on metastable phase α-Ga2O3/ZnO Isotype Heterostructures. ACS Appl Mater Interfaces 2017;9:36997-7005.
31. Wu JY, Chun YT, Li S, et al. Broadband MoS2 field-effect phototransistors: ultrasensitive visible-light photoresponse and negative infrared photoresponse. Adv Mater 2018;30:1705880.
32. Yang Y, Peng X, Kim HS, et al. Hot carrier trapping induced negative photoconductance in inas nanowires toward novel nonvolatile memory. Nano Lett 2015;15:5875-82.
33. Tielrooij KJ, Song JCW, Jensen SA, et al. Photoexcitation cascade and multiple hot-carrier generation in graphene. Nat Phys 2013;9:248-52.
35. Kong WY, Wu GA, Wang KY, et al. Graphene-β-Ga2O3 heterojunction for highly sensitive deep UV Photodetector application. Adv Mater 2016;28:10725-31.
36. Haque MA, Li J, Abdelhady AL, et al. Transition from positive to negative photoconductance in doped hybrid perovskite semiconductors. Adv Opt Mater 2019;7:1900865.
37. Yang X, Ni P, Jing P, et al. Room temperature electrically driven ultraviolet plasmonic lasers. Adv Opt Mater 2019;7:1801681.
38. Yang X, Shan CX, Ni PN, et al. Electrically driven lasers from van der Waals heterostructures. Nanoscale 2018;10:9602-7.
39. Lu Y, Shi Z, Shan C, Shen D. ZnO-based deep-ultraviolet light-emitting devices. Chinese Phys B 2017;26:047703.
40. Shi ZF, Xu TT, Wu D, et al. Semi-transparent all-oxide ultraviolet light-emitting diodes based on ZnO/NiO-core/shell nanowires. Nanoscale 2016;8:9997-10003.
41. Shi ZF, Sun XG, Wu D, et al. High-performance planar green light-emitting diodes based on a PEDOT:PSS/CH3NH3PbBr3/ZnO sandwich structure. Nanoscale 2016;8:10035-42.
42. Guo W, Xu S, Wu Z, Wang N, Loy MM, Du S. Oxygen-assisted charge transfer between ZnO quantum dots and graphene. Small 2013;9:3031-6.
43. Liu X, Yang Y, Xing X, Wang Y. Grey level replaces fluorescent intensity: fluorescent paper sensor based on ZnO nanoparticles for quantitative detection of Cu2+ without photoluminescence spectrometer. Sensor Actuat B Chem 2018;255:2356-66.
44. Barui AK, Veeriah V, Mukherjee S, et al. Zinc oxide nanoflowers make new blood vessels. Nanoscale 2012;4:7861-9.
45. Kim K, Kim H, Choi K, Kim H, Lee J. ZnO hierarchical nanostructures grown at room temperature and their C2H5OH sensor applications. Sensor Actuat B Chem 2011;155:745-51.
46. Pichat P. Powder photocatalysts: characterization by isotopic exchanges and photoconductivity; potentialities for metal recovery, catalyst preparation and water pollutant removal. In Schiavello M. editor, Photocatalysis and environment: trends and applications. Dordrecht: Springer Netherlands. 1988. pp 399-424.
47. Tan Y, Qiao Q, Weng T, et al. Self-powered photodetector based on poly(3-hexylthiophene)/Zinc oxide quantum dots Organic-inorganic hybrid heterojunction. Chem Phys Lett 2022;806:140033.
48. Zhou YH, Zhang ZB, Xu P, Zhang H, Wang B. UV-visible photodetector based on I-type heterostructure of ZnO-QDs/monolayer MoS2. Nanoscale Res Lett 2019;14:364.
49. Zhang J, Zhang X, Ding Y, Zhu Y. ZnO/graphene/Ag composite as recyclable surface-enhanced Raman scattering substrates. Appl Opt 2016;55:9105-12.
50. Zhang BY, Liu T, Meng B, et al. Broadband high photoresponse from pure monolayer graphene photodetector. Nat Commun 2013;4:1811.
51. Zhou H, Qiu C, Yu F, et al. Thickness-dependent morphologies and surface-enhanced raman scattering of Ag deposited on n-layer graphenes. J Phys Chem C 2011;115:11348-54.
52. Wang Q, Tu Y, Ichii T, et al. Decoration of reduced graphene oxide by gold nanoparticles: an enhanced negative photoconductivity. Nanoscale 2017;9:14703-9.
53. Bhatt V, Kumar M, Kim J, Chung H, Yun J. Persistent photoconductivity in Al-doped ZnO photoconductors under air, nitrogen and oxygen ambiance: role of oxygen vacancies induced DX centers. Ceram Int 2019;45:8561-70.
54. Wang Y, Ni Z, Liu L, et al. Stacking-dependent optical conductivity of bilayer graphene. ACS Nano 2010;4:4074-80.
55. Fernando JFS, Zhang C, Firestein K, Nerkar JY, Golberg DV. ZnO quantum dots anchored in multilayered and flexible amorphous carbon sheets for high performance and stable lithium ion batteries. J Mater Chem A 2019;7:8460-71.
56. Zhou Z, Pourhashem S, Wang Z, Duan J, Zhang R, Hou B. Distinctive roles of graphene oxide, ZnO quantum dots, and their nanohybrids in anti-corrosion and anti-fouling performance of waterborne epoxy coatings. Chem Eng J 2022;439:135765.
57. Nowak E, Szybowicz M, Stachowiak A, et al. A comprehensive study of structural and optical properties of ZnO bulk crystals and polycrystalline films grown by sol-gel method. Appl Phys A 2020:126.
58. Kim HH, Lee Y, Lee YJ, et al. Realization of excitation wavelength independent blue emission of ZnO quantum dots with intrinsic defects. ACS Photonics 2020;7:723-34.
59. Han J, Wang J, Yang M, et al. Graphene/Organic semiconductor heterojunction phototransistors with broadband and bi-directional photoresponse. Adv Mater 2018;30:e1804020.
60. Williams G, Kamat PV. Graphene-semiconductor nanocomposites: excited-state interactions between ZnO nanoparticles and graphene oxide. Langmuir 2009;25:13869-73.
61. Li QH, Gao T, Wang YG, Wang TH. Adsorption and desorption of oxygen probed from ZnO nanowire films by photocurrent measurements. Appl Phys Lett 2005;86:123117.
Cite This Article
Yang X, Wang CJ, Cheng S, Yang XG, Zang JH, Shan CX. An ultraviolet-visible distinguishable broadband photodetector based on the positive and negative photoconductance effects of a graphene/ZnO quantum dot heterostructure. Microstructures 2023;3:2023005. http://dx.doi.org/10.20517/microstructures.2022.24
Yang X, Wang CJ, Cheng S, Yang XG, Zang JH, Shan CX. An ultraviolet-visible distinguishable broadband photodetector based on the positive and negative photoconductance effects of a graphene/ZnO quantum dot heterostructure. Microstructures. 2023; 3(1): 2023005. http://dx.doi.org/10.20517/microstructures.2022.24
Yang, Xun, Chao-Jun Wang, Shaobo Cheng, Xi-Gui Yang, Jin-Hao Zang, Chong-Xin Shan. 2023. "An ultraviolet-visible distinguishable broadband photodetector based on the positive and negative photoconductance effects of a graphene/ZnO quantum dot heterostructure" Microstructures. 3, no.1: 2023005. http://dx.doi.org/10.20517/microstructures.2022.24
Yang, X.; Wang C.J.; Cheng S.; Yang X.G.; Zang J.H.; Shan C.X. An ultraviolet-visible distinguishable broadband photodetector based on the positive and negative photoconductance effects of a graphene/ZnO quantum dot heterostructure. Microstructures. 2023, 3, 2023005. http://dx.doi.org/10.20517/microstructures.2022.24
Comments must be written in English. Spam, offensive content, impersonation, and private information will not be permitted. If any comment is reported and identified as inappropriate content by OAE staff, the comment will be removed without notice. If you have any queries or need any help, please contact us at email@example.com.